#------------------------------------------------------------------------------
#$Date: 2021-05-27 10:32:24 +0300 (Thu, 27 May 2021) $
#$Revision: 265541 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/29/1562905.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562905
loop_
_publ_author_name
'Wu, Shuting'
'Deng, Binbin'
'Jiang, Xiuling'
'Li, Ronghua'
'Guo, Jiangbin'
'Lai, Fulong'
'Huang, Xihe'
'Huang, Changcang'
_publ_section_title
;
 Step-by-step assembly of 4d--4f--3d complex based on heptamolybdate anion
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              451
_journal_page_last               457
_journal_paper_doi               10.1016/j.jssc.2012.06.049
_journal_volume                  196
_journal_year                    2012
_chemical_formula_sum            'H0 Mo29 N11 O123 Pr4.7'
_chemical_formula_weight         5566.53
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                100.071(3)
_cell_angle_beta                 92.155(2)
_cell_angle_gamma                113.415(3)
_cell_formula_units_Z            2
_cell_length_a                   17.037(5)
_cell_length_b                   18.917(5)
_cell_length_c                   24.342(6)
_cell_measurement_reflns_used    18413
_cell_measurement_temperature    113(2)
_cell_measurement_theta_max      27.4758
_cell_measurement_theta_min      3.1108
_cell_volume                     7038(3)
_computing_cell_refinement       'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_data_collection       'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC Inc., 2005)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      113(2)
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measured_fraction_theta_full 0.948
_diffrn_measured_fraction_theta_max 0.948
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0397
_diffrn_reflns_av_sigmaI/netI    0.0627
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            44278
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.74
_exptl_absorpt_coefficient_mu    4.283
_exptl_absorpt_correction_T_max  0.3598
_exptl_absorpt_correction_T_min  0.2233
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.647
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             5148
_exptl_crystal_size_max          0.50
_exptl_crystal_size_mid          0.50
_exptl_crystal_size_min          0.30
_refine_diff_density_max         2.363
_refine_diff_density_min         -3.059
_refine_diff_density_rms         0.223
_refine_ls_goodness_of_fit_ref   1.106
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1546
_refine_ls_number_reflns         23514
_refine_ls_number_restraints     24
_refine_ls_restrained_S_all      1.106
_refine_ls_R_factor_all          0.0502
_refine_ls_R_factor_gt           0.0465
_refine_ls_shift/su_max          0.465
_refine_ls_shift/su_mean         0.009
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0857P)²+9.8799P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1438
_refine_ls_wR_factor_ref         0.1479
_reflns_number_gt                20548
_reflns_number_total             23514
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2012-196-451.cif
_cod_data_source_block           1-pr5
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the built-in table derived
from the CIF Core dictionary named 'cif_core.dic' version 2.4.5 last
updated on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1562905
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pr1 Pr 0.94892(3) 0.50452(2) 0.155406(18) 0.01884(11) Uani 1 1 d . . .
Pr2 Pr 0.55329(3) 0.40242(3) 0.309514(19) 0.01980(11) Uani 1 1 d . . .
Pr3 Pr 0.93219(3) 0.63621(2) 0.406203(18) 0.01851(11) Uani 1 1 d . . .
Pr4 Pr 0.66521(3) 0.63839(3) 0.149092(19) 0.01978(11) Uani 1 1 d . . .
Pr5 Pr 1.38374(4) 0.92084(4) 0.21745(3) 0.02380(15) Uani 0.70 1 d P . .
Mo6 Mo 0.77526(4) 0.54489(4) 0.25473(3) 0.01762(15) Uani 1 1 d . . .
Mo7 Mo 0.68303(4) 0.61755(4) 0.41001(3) 0.02134(16) Uani 1 1 d . . .
Mo8 Mo 0.77787(4) 0.40219(4) 0.37916(3) 0.02153(16) Uani 1 1 d . . .
Mo9 Mo 1.04506(4) 0.71083(4) 0.26828(3) 0.01948(15) Uani 1 1 d . . .
Mo10 Mo 0.94608(4) 0.44472(4) 0.31206(3) 0.02013(15) Uani 1 1 d . . .
Mo11 Mo 0.51977(4) 0.29955(4) 0.00971(3) 0.02366(16) Uani 1 1 d . . .
Mo12 Mo 0.89547(5) 0.29561(4) 0.38254(3) 0.02320(16) Uani 1 1 d . . .
Mo13 Mo 0.56702(4) 0.61843(4) 0.30070(3) 0.02255(16) Uani 1 1 d . . .
Mo14 Mo 0.53671(4) 0.40439(4) 0.14041(3) 0.02187(16) Uani 1 1 d . . .
Mo15 Mo 1.12497(4) 0.86577(4) 0.20399(3) 0.02495(17) Uani 1 1 d . . .
Mo16 Mo 0.70715(4) 0.44928(4) 0.07462(3) 0.02109(16) Uani 1 1 d . . .
Mo17 Mo 1.22491(5) 0.85141(4) 0.32381(4) 0.02979(18) Uani 1 1 d . . .
Mo18 Mo 0.93088(4) 0.71392(4) 0.15838(3) 0.02063(16) Uani 1 1 d . . .
Mo19 Mo 0.65668(5) 0.21187(4) 0.02821(3) 0.02987(18) Uani 1 1 d . . .
Mo20 Mo 0.55223(5) 0.71412(4) 0.42887(3) 0.02641(17) Uani 1 1 d . . .
Mo21 Mo 1.05955(5) 0.34419(5) 0.30013(4) 0.0357(2) Uani 1 1 d . . .
Mo22 Mo 0.45577(5) 0.72051(5) 0.30390(4) 0.03318(19) Uani 1 1 d . . .
Mo23 Mo 0.48533(5) 0.16625(4) 0.09329(3) 0.03001(18) Uani 1 1 d . . .
Mo24 Mo 0.64253(5) 0.85840(5) 0.35516(4) 0.03184(19) Uani 1 1 d . . .
Mo25 Mo 0.69705(5) 0.71813(5) 0.53215(3) 0.03066(18) Uani 1 1 d . . .
Mo26 Mo 0.70337(5) 0.25229(5) 0.43552(4) 0.0357(2) Uani 1 1 d . . .
Mo27 Mo 0.75792(5) 0.85802(5) 0.46501(4) 0.03375(19) Uani 1 1 d . . .
Mo28 Mo 0.35892(5) 0.25567(5) 0.09356(4) 0.0345(2) Uani 1 1 d . . .
Mo29 Mo 0.70290(5) 0.16262(5) 0.31011(4) 0.0354(2) Uani 1 1 d . . .
Mo30 Mo 0.98054(5) 0.94738(5) 0.23081(4) 0.0346(2) Uani 1 1 d . . .
Mo31 Mo 0.97887(5) 0.86385(5) 0.10286(4) 0.0353(2) Uani 1 1 d . . .
Mo32 Mo 0.87543(6) 0.20695(5) 0.24475(4) 0.0357(2) Uani 1 1 d . . .
Mo33 Mo 1.10195(5) 0.94507(4) 0.33786(4) 0.03350(19) Uani 1 1 d . . .
Mo34 Mo 0.71157(5) 0.34793(5) -0.04451(3) 0.03156(18) Uani 1 1 d . . .
O1 O 0.5796(3) 0.7321(3) 0.3404(3) 0.0262(13) Uani 1 1 d . . .
O2 O 0.9414(3) 0.7138(3) 0.2386(2) 0.0214(12) Uani 1 1 d . . .
O3 O 0.6811(3) 0.6469(3) 0.3391(2) 0.0230(12) Uani 1 1 d . . .
O4 O 0.8247(3) 0.4102(3) 0.3073(2) 0.0233(12) Uani 1 1 d . . .
O5 O 1.0985(3) 0.8338(3) 0.2895(2) 0.0231(12) Uani 1 1 d . . .
O6 O 0.7919(3) 0.6443(3) 0.4226(2) 0.0272(13) Uani 1 1 d . . .
O7 O 1.0219(4) 0.7015(3) 0.3356(2) 0.0279(13) Uani 1 1 d . . .
O8 O 0.5229(4) 0.3791(4) 0.2051(3) 0.0315(14) Uani 1 1 d . . .
O9 O 0.6540(3) 0.4129(3) 0.1378(2) 0.0213(12) Uani 1 1 d . . .
O10 O 0.8264(3) 0.7057(3) 0.1522(3) 0.0278(13) Uani 1 1 d . . .
O11 O 0.4175(4) 0.3695(4) 0.1095(3) 0.0315(14) Uani 1 1 d . . .
O12 O 0.6000(4) 0.6472(3) 0.2392(2) 0.0277(13) Uani 1 1 d . . .
O13 O 0.8437(4) 0.1951(3) 0.3329(3) 0.0308(14) Uani 1 1 d . . .
O14 O 0.9845(3) 0.8378(3) 0.1855(2) 0.0249(12) Uani 1 1 d . . .
O15 O 0.4968(3) 0.2854(3) 0.0984(2) 0.0231(12) Uani 1 1 d . . .
O16 O 0.8101(3) 0.4571(3) 0.0933(2) 0.0261(13) Uani 1 1 d . . .
O17 O 0.6902(3) 0.7295(3) 0.4461(2) 0.0245(12) Uani 1 1 d . . .
O18 O 0.6600(3) 0.3278(3) 0.0345(2) 0.0248(12) Uani 1 1 d . . .
O19 O 0.5636(4) 0.4042(3) 0.0510(2) 0.0240(12) Uani 1 1 d . . .
O20 O 0.6858(3) 0.4674(3) 0.2702(2) 0.0249(12) Uani 1 1 d . . .
O21 O 1.0726(3) 0.7535(3) 0.1864(2) 0.0224(12) Uani 1 1 d . . .
O22 O 1.1716(3) 0.7458(3) 0.2802(3) 0.0299(14) Uani 1 1 d . . .
O23 O 0.9780(4) 0.5411(3) 0.3496(2) 0.0256(13) Uani 1 1 d . . .
O24 O 0.7600(3) 0.2808(3) 0.3594(3) 0.0255(13) Uani 1 1 d . . .
O25 O 0.9065(3) 0.4002(3) 0.3912(2) 0.0232(12) Uani 1 1 d . . .
O26 O 0.9253(4) 0.6206(3) 0.1348(3) 0.0280(13) Uani 1 1 d . . .
O27 O 0.9680(4) 0.7555(4) 0.0920(3) 0.0326(14) Uani 1 1 d . . .
O28 O 0.7393(3) 0.6029(3) 0.2202(2) 0.0253(12) Uani 1 1 d . . .
O29 O 0.8203(4) 0.5022(3) 0.4079(3) 0.0289(13) Uani 1 1 d . . .
O30 O 0.8418(3) 0.6028(3) 0.3177(2) 0.0250(12) Uani 1 1 d . . .
O31 O 0.5597(4) 0.5037(3) 0.1519(3) 0.0307(14) Uani 1 1 d . . .
O32 O 0.6726(4) 0.3779(3) 0.3523(3) 0.0293(14) Uani 1 1 d . . .
O33 O 0.5165(4) 0.8289(4) 0.3426(3) 0.0377(16) Uani 1 1 d . . .
O34 O 0.6526(4) 0.6136(3) 0.4875(2) 0.0289(13) Uani 1 1 d . . .
O35 O 0.9601(4) 0.4535(4) 0.2431(2) 0.0282(13) Uani 1 1 d . . .
O36 O 0.8351(4) 0.5068(4) 0.2112(2) 0.0268(13) Uani 1 1 d . . .
O37 O 0.9244(4) 0.3237(3) 0.2972(2) 0.0266(13) Uani 1 1 d . . .
O38 O 0.4512(4) 0.6155(4) 0.2952(3) 0.0323(14) Uani 1 1 d . . .
O39 O 0.8211(4) 0.3720(4) -0.0308(3) 0.0420(17) Uani 1 1 d . . .
O40 O 1.0300(4) 0.6169(3) 0.2330(2) 0.0248(12) Uani 1 1 d . . .
O41 O 0.7452(4) 0.8508(4) 0.3837(3) 0.0326(14) Uani 1 1 d . . .
O42 O 1.0030(4) 0.3088(4) 0.3892(3) 0.0310(14) Uani 1 1 d . . .
O43 O 0.7581(4) 0.3655(4) 0.4491(3) 0.0343(15) Uani 1 1 d . . .
O44 O 0.6373(4) 0.5158(3) 0.3874(3) 0.0294(13) Uani 1 1 d . . .
O45 O 0.5342(4) 0.5166(4) 0.2869(3) 0.0330(14) Uani 1 1 d . . .
O46 O 1.0575(4) 0.4425(4) 0.3361(3) 0.0294(13) Uani 1 1 d . . .
O47 O 1.2203(4) 0.9531(3) 0.3417(3) 0.0346(15) Uani 1 1 d . . .
O48 O 0.5506(3) 0.6155(3) 0.3917(3) 0.0255(13) Uani 1 1 d . . .
O49 O 0.8010(4) 0.7295(4) 0.5494(3) 0.0388(16) Uani 1 1 d . . .
O50 O 0.6105(4) 0.2089(3) 0.0997(2) 0.0290(13) Uani 1 1 d . . .
O51 O 0.5204(4) 0.1994(3) 0.0108(2) 0.0293(13) Uani 1 1 d . . .
O52 O 0.8574(4) 0.2699(4) 0.4441(3) 0.0331(14) Uani 1 1 d . . .
O53 O 1.0118(4) 0.9630(4) 0.1551(3) 0.0400(16) Uani 1 1 d . . .
O54 O 0.6168(4) 0.8243(4) 0.4387(3) 0.0349(15) Uani 1 1 d . . .
O55 O 0.7191(4) 0.8266(4) 0.5344(3) 0.0385(16) Uani 1 1 d . . .
O56 O 1.1159(4) 0.9556(3) 0.2470(3) 0.0306(14) Uani 1 1 d . . .
O57 O 0.9847(4) 0.9101(3) 0.2990(3) 0.0326(14) Uani 1 1 d . . .
O58 O 0.7602(4) 0.2057(4) 0.2491(3) 0.0357(15) Uani 1 1 d . . .
O59 O 0.7143(4) 0.5448(3) 0.0910(3) 0.0294(13) Uani 1 1 d . . .
O60 O 0.7119(4) 0.4468(4) -0.0071(2) 0.0317(14) Uani 1 1 d . . .
O61 O 1.2166(5) 0.8287(4) 0.3888(3) 0.0488(18) Uani 1 1 d . . .
O62 O 0.6931(4) 0.1545(4) 0.3902(3) 0.0400(16) Uani 1 1 d . . .
O63 O 1.2304(4) 0.8830(3) 0.2292(3) 0.0330(14) Uani 1 1 d . . .
O64 O 0.8728(4) 0.3578(4) 0.1386(3) 0.0410(16) Uani 1 1 d . . .
O65 O 0.6819(5) 0.0650(4) 0.2889(3) 0.0505(19) Uani 1 1 d . . .
O66 O 0.9415(4) 0.7729(4) 0.4108(3) 0.0386(16) Uani 1 1 d . . .
O67 O 0.4672(5) 0.7323(5) 0.2360(3) 0.0478(18) Uani 1 1 d . . .
O68 O 0.6240(5) 0.1121(4) 0.0021(3) 0.0459(18) Uani 1 1 d . . .
O69 O 0.5990(4) 0.2421(4) 0.4234(3) 0.0500(19) Uani 1 1 d . . .
O70 O 1.0883(4) 0.7193(5) 0.4429(3) 0.057(2) Uani 1 1 d . . .
O71 O 1.3324(4) 0.8775(4) 0.3131(3) 0.0422(17) Uani 1 1 d . . .
O72 O 0.9948(4) 0.2318(4) 0.2752(3) 0.0409(16) Uani 1 1 d . . .
O73 O 0.4606(5) 0.0706(4) 0.0644(3) 0.0479(18) Uani 1 1 d . . .
O74 O 0.5540(5) 0.2749(4) 0.2612(3) 0.0448(17) Uani 1 1 d . . .
O75 O 0.6693(4) 0.2363(4) -0.0483(3) 0.0356(15) Uani 1 1 d . . .
O76 O 1.0882(4) 0.6080(4) 0.1288(3) 0.0394(16) Uani 1 1 d . . .
O77 O 0.9653(5) 0.4595(5) 0.0552(3) 0.0509(19) Uani 1 1 d . . .
O78 O 0.3966(4) 0.3160(5) 0.2725(3) 0.058(2) Uani 1 1 d . . .
O79 O 0.6056(4) 0.1680(4) 0.2928(4) 0.052(2) Uani 1 1 d . . .
O80 O 0.8694(4) 0.9109(4) 0.2170(4) 0.052(2) Uani 1 1 d . . .
O81 O 0.7265(4) 0.7757(4) 0.2084(3) 0.0453(18) Uani 1 1 d . . .
O82 O 0.5671(4) 0.5788(4) 0.0580(3) 0.0417(17) Uani 1 1 d . . .
O83 O 0.6675(4) 0.8603(4) 0.2874(3) 0.0458(18) Uani 1 1 d . . .
O84 O 0.3691(4) 0.1572(4) 0.0680(3) 0.0375(15) Uani 1 1 d . . .
O85 O 0.7643(4) 0.2463(4) 0.0536(3) 0.0430(17) Uani 1 1 d . . .
O86 O 0.8725(4) 0.8434(4) 0.0833(3) 0.0493(19) Uani 1 1 d . . .
O87 O 0.8573(4) 0.8542(4) 0.4697(3) 0.0429(17) Uani 1 1 d . . .
O88 O 0.5545(4) 0.3136(4) -0.0556(3) 0.0335(14) Uani 1 1 d . . .
O89 O 0.4099(4) 0.2757(4) 0.0014(3) 0.0370(15) Uani 1 1 d . . .
O90 O 0.4502(4) 0.7045(4) 0.4051(3) 0.0432(17) Uani 1 1 d . . .
O91 O 0.9892(4) 0.5758(4) 0.4736(3) 0.0444(17) Uani 1 1 d . . .
O92 O 1.0690(5) 0.9087(4) 0.3966(3) 0.0463(18) Uani 1 1 d . . .
O93 O 0.7123(5) 0.2344(5) 0.5021(3) 0.052(2) Uani 1 1 d . . .
O94 O 0.6483(4) 0.7047(5) 0.5921(3) 0.0454(18) Uani 1 1 d . . .
O95 O 0.6644(5) 0.9552(4) 0.3843(3) 0.0462(18) Uani 1 1 d . . .
O96 O 0.3343(5) 0.2436(4) 0.1600(3) 0.0491(19) Uani 1 1 d . . .
O97 O 0.4762(5) 0.1689(4) 0.1640(3) 0.0410(16) Uani 1 1 d . . .
O98 O 0.2640(4) 0.2405(5) 0.0555(3) 0.060(2) Uani 1 1 d . . .
O99 O 0.5420(5) 0.6798(5) 0.1458(3) 0.051(2) Uani 1 1 d . . .
O100 O 0.7783(5) 0.9549(4) 0.4876(3) 0.0493(19) Uani 1 1 d . . .
O101 O 0.5482(4) 0.7022(4) 0.4980(3) 0.0401(16) Uani 1 1 d . . .
O102 O 1.1312(4) 0.8872(4) 0.1378(3) 0.0369(15) Uani 1 1 d . . .
O103 O 0.8492(6) 0.1073(4) 0.2252(3) 0.056(2) Uani 1 1 d . . .
O104 O 1.0690(5) 0.4590(5) 0.1596(3) 0.053(2) Uani 1 1 d . . .
O105 O 1.0135(5) 1.0457(4) 0.2565(4) 0.054(2) Uani 1 1 d . . .
O106 O 0.8932(5) 0.2413(4) 0.1837(3) 0.0488(18) Uani 1 1 d . . .
O107 O 0.7100(4) 0.7221(5) 0.0777(3) 0.051(2) Uani 1 1 d . . .
O108 O 0.5081(4) 0.3169(5) 0.3795(4) 0.055(2) Uani 1 1 d . . .
O109 O 1.1304(5) 1.0436(4) 0.3558(4) 0.053(2) Uani 1 1 d . . .
O110 O 1.0894(5) 0.3682(5) 0.2374(3) 0.056(2) Uani 1 1 d . . .
O111 O 1.1504(5) 0.3463(5) 0.3353(4) 0.059(2) Uani 1 1 d . . .
O112 O 0.6956(5) 0.3507(4) -0.1147(3) 0.0504(19) Uani 1 1 d . . .
O113 O 0.3505(4) 0.7051(4) 0.3119(3) 0.0500(19) Uani 1 1 d . . .
O114 O 0.4542(5) 0.4457(5) 0.3738(3) 0.053(2) Uani 1 1 d . . .
O115 O 1.0307(5) 0.8922(5) 0.0470(3) 0.053(2) Uani 1 1 d . . .
O116 O 0.9250(5) 0.6897(6) 0.5076(3) 0.063(2) Uani 1 1 d . . .
O117 O 1.5143(6) 0.9248(6) 0.2667(5) 0.086(3) Uani 1 1 d . . .
O118 O 1.5098(6) 1.0279(6) 0.1894(5) 0.083(3) Uani 1 1 d . . .
O119 O 1.3135(8) 0.8885(8) 0.1198(4) 0.105(4) Uani 1 1 d . . .
O120 O 1.4402(7) 1.0348(6) 0.3006(5) 0.097(4) Uani 1 1 d . . .
O121 O 1.3106(6) 0.7734(6) 0.2062(4) 0.073(3) Uani 1 1 d . . .
O122 O 1.4541(7) 0.8549(7) 0.1466(5) 0.097(3) Uani 1 1 d . . .
O123 O 1.3458(6) 1.0328(6) 0.1990(6) 0.100(4) Uani 1 1 d . . .
N1 N 0.7153(5) 0.3231(5) 0.2018(4) 0.0400(19) Uani 1 1 d . . .
N2 N 0.8883(6) 0.4874(6) 0.5472(4) 0.059(3) Uani 1 1 d . . .
N3 N 0.6091(7) 0.5221(7) -0.0459(5) 0.066(3) Uani 1 1 d . . .
N4 N 0.8322(5) 0.7676(5) 0.3096(4) 0.042(2) Uani 1 1 d . . .
N5 N 0.953(2) 0.8388(19) 0.6468(11) 0.150(13) Uani 0.74 1 d P . .
N5A N 0.922(5) 0.829(2) 0.646(2) 0.10(4) Uani 0.26 1 d P . .
N6 N 0.4113(8) 0.8617(7) 0.4271(5) 0.082(4) Uani 1 1 d . . .
N7 N 0.5535(7) -0.0343(6) 0.0616(5) 0.070(3) Uani 1 1 d . . .
N8 N 1.0000 1.0000 0.5000 0.147(11) Uani 1 2 d S . .
N8A N 0.707(3) 1.0091(18) 0.9680(18) 0.21(3) Uani 0.50 1 d P . .
N9 N 0.1746(9) 0.5868(11) 0.2958(11) 0.126(8) Uani 0.86 1 d PU . .
N9A N 0.180(3) 0.634(4) 0.356(4) 0.06(2) Uani 0.14 1 d PU . .
N10 N 1.5274(11) 1.0253(10) 0.3976(7) 0.116(5) Uani 1 1 d . . .
N11 N 0.6521(12) 0.8989(13) 0.6110(8) 0.086(8) Uani 0.77 1 d PU . .
N11A N 0.672(4) 0.905(4) 0.638(3) 0.08(2) Uani 0.23 1 d PU . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O36 Pr1 O40 78.97(19) . .
O36 Pr1 O16 69.90(18) . .
O40 Pr1 O16 136.06(18) . .
O36 Pr1 O77 138.3(2) . .
O40 Pr1 O77 137.0(2) . .
O16 Pr1 O77 68.6(2) . .
O36 Pr1 O64 86.0(2) . .
O40 Pr1 O64 139.2(2) . .
O16 Pr1 O64 69.5(2) . .
O77 Pr1 O64 76.1(2) . .
O36 Pr1 O26 77.07(19) . .
O40 Pr1 O26 72.91(19) . .
O16 Pr1 O26 70.51(19) . .
O77 Pr1 O26 92.8(2) . .
O64 Pr1 O26 139.8(2) . .
O36 Pr1 O35 69.89(18) . .
O40 Pr1 O35 71.09(19) . .
O16 Pr1 O35 122.34(19) . .
O77 Pr1 O35 132.4(2) . .
O64 Pr1 O35 68.2(2) . .
O26 Pr1 O35 134.71(19) . .
O36 Pr1 O104 137.0(2) . .
O40 Pr1 O104 89.7(2) . .
O16 Pr1 O104 134.1(2) . .
O77 Pr1 O104 74.6(2) . .
O64 Pr1 O104 75.9(2) . .
O26 Pr1 O104 138.8(2) . .
O35 Pr1 O104 67.2(2) . .
O36 Pr1 O76 136.5(2) . .
O40 Pr1 O76 66.0(2) . .
O16 Pr1 O76 119.6(2) . .
O77 Pr1 O76 71.0(2) . .
O64 Pr1 O76 137.5(2) . .
O26 Pr1 O76 68.7(2) . .
O35 Pr1 O76 118.1(2) . .
O104 Pr1 O76 70.1(2) . .
O20 Pr2 O45 78.52(19) . .
O20 Pr2 O44 77.8(2) . .
O45 Pr2 O44 73.7(2) . .
O20 Pr2 O108 136.0(2) . .
O45 Pr2 O108 137.8(2) . .
O44 Pr2 O108 89.1(3) . .
O20 Pr2 O32 69.41(18) . .
O45 Pr2 O32 136.37(19) . .
O44 Pr2 O32 71.29(19) . .
O108 Pr2 O32 66.6(2) . .
O20 Pr2 O74 87.2(2) . .
O45 Pr2 O74 139.9(2) . .
O44 Pr2 O74 139.5(2) . .
O108 Pr2 O74 75.9(3) . .
O32 Pr2 O74 68.2(2) . .
O20 Pr2 O8 70.35(19) . .
O45 Pr2 O8 72.2(2) . .
O44 Pr2 O8 137.0(2) . .
O108 Pr2 O8 133.9(3) . .
O32 Pr2 O8 120.4(2) . .
O74 Pr2 O8 67.7(2) . .
O20 Pr2 O78 136.9(2) . .
O45 Pr2 O78 89.7(2) . .
O44 Pr2 O78 138.3(2) . .
O108 Pr2 O78 77.9(3) . .
O32 Pr2 O78 133.9(2) . .
O74 Pr2 O78 75.5(3) . .
O8 Pr2 O78 66.6(2) . .
O20 Pr2 O114 136.6(2) . .
O45 Pr2 O114 67.2(2) . .
O44 Pr2 O114 67.8(2) . .
O108 Pr2 O114 70.6(2) . .
O32 Pr2 O114 119.8(2) . .
O74 Pr2 O114 136.2(2) . .
O8 Pr2 O114 119.7(2) . .
O78 Pr2 O114 70.5(3) . .
O30 Pr3 O23 78.92(19) . .
O30 Pr3 O6 69.28(19) . .
O23 Pr3 O6 135.92(19) . .
O30 Pr3 O7 70.75(19) . .
O23 Pr3 O7 71.68(19) . .
O6 Pr3 O7 121.78(19) . .
O30 Pr3 O29 77.50(19) . .
O23 Pr3 O29 73.63(18) . .
O6 Pr3 O29 70.35(18) . .
O7 Pr3 O29 136.5(2) . .
O30 Pr3 O66 85.2(2) . .
O23 Pr3 O66 139.6(2) . .
O6 Pr3 O66 68.15(19) . .
O7 Pr3 O66 68.0(2) . .
O29 Pr3 O66 138.38(19) . .
O30 Pr3 O70 136.2(2) . .
O23 Pr3 O70 88.1(3) . .
O6 Pr3 O70 135.9(3) . .
O7 Pr3 O70 65.5(2) . .
O29 Pr3 O70 138.2(2) . .
O66 Pr3 O70 78.1(3) . .
O30 Pr3 O91 142.1(2) . .
O23 Pr3 O91 72.7(2) . .
O6 Pr3 O91 116.6(2) . .
O7 Pr3 O91 121.1(2) . .
O29 Pr3 O91 70.8(2) . .
O66 Pr3 O91 132.5(2) . .
O70 Pr3 O91 68.0(2) . .
O30 Pr3 O116 135.7(2) . .
O23 Pr3 O116 140.1(2) . .
O6 Pr3 O116 66.8(2) . .
O7 Pr3 O116 130.6(3) . .
O29 Pr3 O116 92.9(3) . .
O66 Pr3 O116 73.6(3) . .
O70 Pr3 O116 77.3(3) . .
O91 Pr3 O116 67.4(2) . .
O28 Pr4 O31 78.06(19) . .
O28 Pr4 O107 135.7(2) . .
O31 Pr4 O107 137.1(2) . .
O28 Pr4 O59 77.79(19) . .
O31 Pr4 O59 73.23(19) . .
O107 Pr4 O59 87.7(2) . .
O28 Pr4 O12 70.11(18) . .
O31 Pr4 O12 72.7(2) . .
O107 Pr4 O12 135.3(2) . .
O59 Pr4 O12 137.00(18) . .
O28 Pr4 O81 87.2(2) . .
O31 Pr4 O81 139.9(2) . .
O107 Pr4 O81 77.4(3) . .
O59 Pr4 O81 139.8(2) . .
O12 Pr4 O81 67.1(2) . .
O28 Pr4 O99 135.3(2) . .
O31 Pr4 O99 88.5(2) . .
O107 Pr4 O99 81.0(3) . .
O59 Pr4 O99 138.5(2) . .
O12 Pr4 O99 65.2(2) . .
O81 Pr4 O99 76.1(2) . .
O28 Pr4 O82 141.1(2) . .
O31 Pr4 O82 70.3(2) . .
O107 Pr4 O82 67.4(2) . .
O59 Pr4 O82 71.9(2) . .
O12 Pr4 O82 118.8(2) . .
O81 Pr4 O82 131.6(2) . .
O99 Pr4 O82 66.8(2) . .
O28 Pr4 O10 68.27(18) . .
O31 Pr4 O10 135.66(18) . .
O107 Pr4 O10 67.4(2) . .
O59 Pr4 O10 72.14(19) . .
O12 Pr4 O10 118.49(19) . .
O81 Pr4 O10 67.6(2) . .
O99 Pr4 O10 135.8(2) . .
O82 Pr4 O10 122.2(2) . .
O117 Pr5 O63 139.2(3) . .
O117 Pr5 O119 138.6(4) . .
O63 Pr5 O119 76.5(3) . .
O117 Pr5 O118 73.0(3) . .
O63 Pr5 O118 141.1(3) . .
O119 Pr5 O118 87.9(4) . .
O117 Pr5 O121 91.3(3) . .
O63 Pr5 O121 71.1(2) . .
O119 Pr5 O121 81.6(4) . .
O118 Pr5 O121 142.1(3) . .
O117 Pr5 O120 70.1(4) . .
O63 Pr5 O120 95.9(3) . .
O119 Pr5 O120 139.2(4) . .
O118 Pr5 O120 73.1(4) . .
O121 Pr5 O120 134.3(3) . .
O117 Pr5 O123 130.2(4) . .
O63 Pr5 O123 72.7(3) . .
O119 Pr5 O123 70.1(4) . .
O118 Pr5 O123 68.5(3) . .
O121 Pr5 O123 138.2(3) . .
O120 Pr5 O123 69.4(4) . .
O117 Pr5 O122 71.9(4) . .
O63 Pr5 O122 129.6(3) . .
O119 Pr5 O122 67.3(4) . .
O118 Pr5 O122 72.3(4) . .
O121 Pr5 O122 70.0(3) . .
O120 Pr5 O122 134.4(3) . .
O123 Pr5 O122 121.9(4) . .
O117 Pr5 O71 76.6(3) . .
O63 Pr5 O71 62.7(2) . .
O119 Pr5 O71 134.7(3) . .
O118 Pr5 O71 136.5(3) . .
O121 Pr5 O71 67.6(2) . .
O120 Pr5 O71 67.6(3) . .
O123 Pr5 O71 112.3(3) . .
O122 Pr5 O71 125.7(3) . .
O20 Mo6 O36 109.7(3) . .
O20 Mo6 O28 109.1(3) . .
O36 Mo6 O28 109.7(3) . .
O20 Mo6 O30 109.6(3) . .
O36 Mo6 O30 108.7(3) . .
O28 Mo6 O30 110.1(3) . .
O6 Mo7 O44 105.8(3) . .
O6 Mo7 O3 98.2(3) . .
O44 Mo7 O3 99.1(3) . .
O6 Mo7 O34 99.3(3) . .
O44 Mo7 O34 94.0(3) . .
O3 Mo7 O34 154.3(2) . .
O6 Mo7 O17 94.3(2) . .
O44 Mo7 O17 157.8(2) . .
O3 Mo7 O17 86.9(2) . .
O34 Mo7 O17 73.3(2) . .
O6 Mo7 O48 165.0(2) . .
O44 Mo7 O48 88.2(2) . .
O3 Mo7 O48 73.9(2) . .
O34 Mo7 O48 84.7(2) . .
O17 Mo7 O48 72.9(2) . .
O6 Mo7 Mo25 86.9(2) . .
O44 Mo7 Mo25 128.5(2) . .
O3 Mo7 Mo25 128.88(17) . .
O34 Mo7 Mo25 34.51(17) . .
O17 Mo7 Mo25 42.03(16) . .
O48 Mo7 Mo25 88.41(15) . .
O32 Mo8 O29 105.5(3) . .
O32 Mo8 O43 100.0(3) . .
O29 Mo8 O43 97.3(3) . .
O32 Mo8 O4 95.5(3) . .
O29 Mo8 O4 97.1(3) . .
O43 Mo8 O4 155.2(2) . .
O32 Mo8 O24 91.8(2) . .
O29 Mo8 O24 162.0(2) . .
O43 Mo8 O24 74.4(2) . .
O4 Mo8 O24 85.9(2) . .
O32 Mo8 O25 161.3(3) . .
O29 Mo8 O25 91.2(2) . .
O43 Mo8 O25 86.0(2) . .
O4 Mo8 O25 73.6(2) . .
O24 Mo8 O25 72.6(2) . .
O32 Mo8 Mo26 87.10(18) . .
O29 Mo8 Mo26 131.5(2) . .
O43 Mo8 Mo26 34.3(2) . .
O4 Mo8 Mo26 128.67(16) . .
O24 Mo8 Mo26 42.77(16) . .
O25 Mo8 Mo26 88.11(14) . .
O7 Mo9 O40 105.5(3) . .
O7 Mo9 O2 99.7(2) . .
O40 Mo9 O2 99.4(2) . .
O7 Mo9 O22 99.2(3) . .
O40 Mo9 O22 92.1(2) . .
O2 Mo9 O22 154.3(2) . .
O7 Mo9 O5 93.1(3) . .
O40 Mo9 O5 158.1(2) . .
O2 Mo9 O5 88.4(2) . .
O22 Mo9 O5 73.3(2) . .
O7 Mo9 O21 165.1(2) . .
O40 Mo9 O21 89.0(2) . .
O2 Mo9 O21 73.7(2) . .
O22 Mo9 O21 83.7(2) . .
O5 Mo9 O21 73.6(2) . .
O7 Mo9 Mo17 87.1(2) . .
O40 Mo9 Mo17 126.28(18) . .
O2 Mo9 Mo17 130.24(17) . .
O22 Mo9 Mo17 34.25(17) . .
O5 Mo9 Mo17 41.86(15) . .
O21 Mo9 Mo17 87.23(14) . .
O35 Mo10 O23 104.9(3) . .
O35 Mo10 O4 99.2(3) . .
O23 Mo10 O4 99.9(2) . .
O35 Mo10 O46 99.6(3) . .
O23 Mo10 O46 92.2(3) . .
O4 Mo10 O46 154.2(2) . .
O35 Mo10 O37 94.6(3) . .
O23 Mo10 O37 157.8(2) . .
O4 Mo10 O37 87.1(2) . .
O46 Mo10 O37 73.9(2) . .
O35 Mo10 O25 165.0(2) . .
O23 Mo10 O25 89.5(2) . .
O4 Mo10 O25 73.7(2) . .
O46 Mo10 O25 83.8(2) . .
O37 Mo10 O25 72.1(2) . .
O89 Mo11 O88 105.8(3) . .
O89 Mo11 O19 101.6(3) . .
O88 Mo11 O19 101.4(3) . .
O89 Mo11 O51 101.2(3) . .
O88 Mo11 O51 100.8(3) . .
O19 Mo11 O51 142.2(2) . .
O89 Mo11 O15 83.3(3) . .
O88 Mo11 O15 170.9(2) . .
O19 Mo11 O15 76.5(2) . .
O51 Mo11 O15 76.8(2) . .
O89 Mo11 O18 171.0(3) . .
O88 Mo11 O18 83.2(2) . .
O19 Mo11 O18 76.4(2) . .
O51 Mo11 O18 76.3(2) . .
O15 Mo11 O18 87.7(2) . .
O52 Mo12 O42 105.4(3) . .
O52 Mo12 O25 102.9(3) . .
O42 Mo12 O25 101.7(3) . .
O52 Mo12 O13 99.7(3) . .
O42 Mo12 O13 100.7(3) . .
O25 Mo12 O13 142.3(2) . .
O52 Mo12 O24 83.9(2) . .
O42 Mo12 O24 170.6(2) . .
O25 Mo12 O24 77.0(2) . .
O13 Mo12 O24 76.0(2) . .
O52 Mo12 O37 171.4(2) . .
O42 Mo12 O37 83.0(2) . .
O25 Mo12 O37 76.6(2) . .
O13 Mo12 O37 76.6(2) . .
O24 Mo12 O37 87.7(2) . .
O12 Mo13 O45 105.6(3) . .
O12 Mo13 O3 97.1(2) . .
O45 Mo13 O3 97.4(2) . .
O12 Mo13 O38 100.5(3) . .
O45 Mo13 O38 95.8(3) . .
O3 Mo13 O38 154.3(3) . .
O12 Mo13 O1 93.4(3) . .
O45 Mo13 O1 159.9(3) . .
O3 Mo13 O1 86.5(2) . .
O38 Mo13 O1 73.9(2) . .
O12 Mo13 O48 163.8(2) . .
O45 Mo13 O48 88.9(2) . .
O3 Mo13 O48 73.5(2) . .
O38 Mo13 O48 84.9(2) . .
O1 Mo13 O48 73.3(2) . .
O12 Mo13 Mo22 87.50(18) . .
O45 Mo13 Mo22 130.19(19) . .
O3 Mo13 Mo22 129.05(16) . .
O38 Mo13 Mo22 34.43(18) . .
O1 Mo13 Mo22 42.54(15) . .
O48 Mo13 Mo22 88.56(13) . .
O8 Mo14 O31 105.9(3) . .
O8 Mo14 O11 100.5(3) . .
O31 Mo14 O11 95.4(3) . .
O8 Mo14 O9 97.2(3) . .
O31 Mo14 O9 97.8(2) . .
O11 Mo14 O9 154.1(2) . .
O8 Mo14 O15 92.3(3) . .
O31 Mo14 O15 160.5(3) . .
O11 Mo14 O15 74.1(2) . .
O9 Mo14 O15 86.4(2) . .
O8 Mo14 O19 162.2(2) . .
O31 Mo14 O19 90.5(3) . .
O11 Mo14 O19 84.4(2) . .
O9 Mo14 O19 73.3(2) . .
O15 Mo14 O19 72.4(2) . .
O8 Mo14 Mo28 87.1(2) . .
O31 Mo14 Mo28 129.73(19) . .
O11 Mo14 Mo28 34.42(18) . .
O9 Mo14 Mo28 129.12(16) . .
O15 Mo14 Mo28 42.67(14) . .
O19 Mo14 Mo28 87.52(15) . .
O102 Mo15 O63 105.5(3) . .
O102 Mo15 O56 101.8(3) . .
O63 Mo15 O56 100.0(3) . .
O102 Mo15 O21 101.4(3) . .
O63 Mo15 O21 100.7(3) . .
O56 Mo15 O21 143.2(2) . .
O102 Mo15 O14 84.0(3) . .
O63 Mo15 O14 170.5(3) . .
O56 Mo15 O14 77.7(2) . .
O21 Mo15 O14 76.7(2) . .
O102 Mo15 O5 172.7(2) . .
O63 Mo15 O5 81.8(3) . .
O56 Mo15 O5 76.5(2) . .
O21 Mo15 O5 76.8(2) . .
O14 Mo15 O5 88.7(2) . .
O59 Mo16 O16 105.1(3) . .
O59 Mo16 O9 98.5(3) . .
O16 Mo16 O9 99.2(2) . .
O59 Mo16 O60 94.7(3) . .
O16 Mo16 O60 99.3(3) . .
O9 Mo16 O60 153.5(2) . .
O59 Mo16 O18 159.2(3) . .
O16 Mo16 O18 94.0(2) . .
O9 Mo16 O18 86.1(2) . .
O60 Mo16 O18 73.8(2) . .
O59 Mo16 O19 89.8(2) . .
O16 Mo16 O19 164.3(2) . .
O9 Mo16 O19 73.5(2) . .
O60 Mo16 O19 83.8(2) . .
O18 Mo16 O19 72.0(2) . .
O59 Mo16 Mo34 129.1(2) . .
O16 Mo16 Mo34 87.12(19) . .
O9 Mo16 Mo34 128.57(17) . .
O60 Mo16 Mo34 34.46(17) . .
O18 Mo16 Mo34 42.43(15) . .
O19 Mo16 Mo34 86.94(14) . .
O61 Mo17 O71 105.8(4) . .
O61 Mo17 O22 97.6(3) . .
O71 Mo17 O22 101.6(3) . .
O61 Mo17 O47 99.2(3) . .
O71 Mo17 O47 101.6(3) . .
O22 Mo17 O47 146.3(3) . .
O61 Mo17 O5 107.5(3) . .
O71 Mo17 O5 146.6(3) . .
O22 Mo17 O5 73.0(2) . .
O47 Mo17 O5 74.1(2) . .
O61 Mo17 O63 177.6(3) . .
O71 Mo17 O63 76.6(3) . .
O22 Mo17 O63 81.7(2) . .
O47 Mo17 O63 80.3(2) . .
O5 Mo17 O63 70.1(2) . .
O61 Mo17 Mo9 94.5(2) . .
O71 Mo17 Mo9 135.5(2) . .
O22 Mo17 Mo9 35.50(16) . .
O47 Mo17 Mo9 113.90(18) . .
O5 Mo17 Mo9 40.31(14) . .
O63 Mo17 Mo9 83.69(14) . .
O26 Mo18 O10 106.2(3) . .
O26 Mo18 O27 97.9(3) . .
O10 Mo18 O27 99.2(3) . .
O26 Mo18 O2 96.7(3) . .
O10 Mo18 O2 97.2(2) . .
O27 Mo18 O2 154.0(2) . .
O26 Mo18 O14 159.6(2) . .
O10 Mo18 O14 93.9(2) . .
O27 Mo18 O14 74.6(2) . .
O2 Mo18 O14 84.3(2) . .
O26 Mo18 O21 88.2(2) . .
O10 Mo18 O21 163.8(2) . .
O27 Mo18 O21 85.8(2) . .
O2 Mo18 O21 73.3(2) . .
O14 Mo18 O21 72.5(2) . .
O26 Mo18 Mo31 133.2(2) . .
O10 Mo18 Mo31 86.65(19) . .
O27 Mo18 Mo31 35.28(18) . .
O2 Mo18 Mo31 126.74(16) . .
O14 Mo18 Mo31 42.48(16) . .
O21 Mo18 Mo31 88.79(14) . .
O85 Mo19 O68 105.4(3) . .
O85 Mo19 O50 97.8(3) . .
O68 Mo19 O50 100.0(3) . .
O85 Mo19 O75 99.3(3) . .
O68 Mo19 O75 92.3(3) . .
O50 Mo19 O75 155.4(2) . .
O85 Mo19 O18 93.9(3) . .
O68 Mo19 O18 157.7(3) . .
O50 Mo19 O18 88.3(2) . .
O75 Mo19 O18 73.1(2) . .
O85 Mo19 O51 163.7(3) . .
O68 Mo19 O51 90.2(3) . .
O50 Mo19 O51 74.3(2) . .
O75 Mo19 O51 84.6(2) . .
O18 Mo19 O51 72.0(2) . .
O101 Mo20 O90 106.0(3) . .
O101 Mo20 O54 101.6(3) . .
O90 Mo20 O54 101.4(3) . .
O101 Mo20 O48 101.1(3) . .
O90 Mo20 O48 101.4(3) . .
O54 Mo20 O48 141.8(2) . .
O101 Mo20 O17 83.0(3) . .
O90 Mo20 O17 171.0(3) . .
O54 Mo20 O17 76.3(2) . .
O48 Mo20 O17 76.4(2) . .
O101 Mo20 O1 170.9(2) . .
O90 Mo20 O1 83.1(3) . .
O54 Mo20 O1 76.2(2) . .
O48 Mo20 O1 76.5(2) . .
O17 Mo20 O1 87.9(2) . .
O110 Mo21 O111 105.2(4) . .
O110 Mo21 O72 99.4(4) . .
O111 Mo21 O72 100.3(3) . .
O110 Mo21 O46 98.3(3) . .
O111 Mo21 O46 102.3(3) . .
O72 Mo21 O46 146.4(3) . .
O110 Mo21 O37 105.2(3) . .
O111 Mo21 O37 149.6(3) . .
O72 Mo21 O37 73.8(2) . .
O46 Mo21 O37 74.0(2) . .
O110 Mo21 O42 174.8(3) . .
O111 Mo21 O42 79.9(3) . .
O72 Mo21 O42 79.7(3) . .
O46 Mo21 O42 80.1(2) . .
O37 Mo21 O42 69.7(2) . .
O67 Mo22 O113 104.9(4) . .
O67 Mo22 O33 99.3(3) . .
O113 Mo22 O33 101.3(3) . .
O67 Mo22 O38 99.0(3) . .
O113 Mo22 O38 102.2(3) . .
O33 Mo22 O38 145.2(3) . .
O67 Mo22 O1 106.5(3) . .
O113 Mo22 O1 148.6(3) . .
O33 Mo22 O1 73.5(2) . .
O38 Mo22 O1 73.1(2) . .
O67 Mo22 Mo13 94.1(2) . .
O113 Mo22 Mo13 136.1(3) . .
O33 Mo22 Mo13 114.36(19) . .
O38 Mo22 Mo13 34.85(17) . .
O1 Mo22 Mo13 41.29(15) . .
O73 Mo23 O97 105.2(3) . .
O73 Mo23 O50 100.3(3) . .
O97 Mo23 O50 96.8(3) . .
O73 Mo23 O84 92.6(3) . .
O97 Mo23 O84 99.3(3) . .
O50 Mo23 O84 156.0(2) . .
O73 Mo23 O15 158.2(3) . .
O97 Mo23 O15 94.0(3) . .
O50 Mo23 O15 87.4(2) . .
O84 Mo23 O15 73.8(2) . .
O73 Mo23 O51 90.2(3) . .
O97 Mo23 O51 163.6(3) . .
O50 Mo23 O51 74.4(2) . .
O84 Mo23 O51 85.5(2) . .
O15 Mo23 O51 72.2(2) . .
O83 Mo24 O95 104.1(4) . .
O83 Mo24 O41 96.2(3) . .
O95 Mo24 O41 101.0(3) . .
O83 Mo24 O33 99.9(3) . .
O95 Mo24 O33 92.7(3) . .
O41 Mo24 O33 155.6(3) . .
O83 Mo24 O1 94.3(3) . .
O95 Mo24 O1 158.4(3) . .
O41 Mo24 O1 87.9(2) . .
O33 Mo24 O1 72.8(2) . .
O83 Mo24 O54 163.5(3) . .
O95 Mo24 O54 91.1(3) . .
O41 Mo24 O54 74.3(2) . .
O33 Mo24 O54 85.4(2) . .
O1 Mo24 O54 72.2(2) . .
O94 Mo25 O49 105.4(3) . .
O94 Mo25 O34 102.7(3) . .
O49 Mo25 O34 98.7(3) . .
O94 Mo25 O55 100.1(3) . .
O49 Mo25 O55 98.8(3) . .
O34 Mo25 O55 146.3(3) . .
O94 Mo25 O17 149.3(3) . .
O49 Mo25 O17 105.3(3) . .
O34 Mo25 O17 73.5(2) . .
O55 Mo25 O17 74.2(3) . .
O94 Mo25 Mo7 137.7(3) . .
O49 Mo25 Mo7 92.8(2) . .
O34 Mo25 Mo7 35.91(17) . .
O55 Mo25 Mo7 114.7(2) . .
O17 Mo25 Mo7 40.92(15) . .
O94 Mo25 Mo27 133.9(3) . .
O49 Mo25 Mo27 92.8(2) . .
O34 Mo25 Mo27 116.16(17) . .
O55 Mo25 Mo27 34.4(2) . .
O17 Mo25 Mo27 43.04(15) . .
Mo7 Mo25 Mo27 81.26(3) . .
O69 Mo26 O93 104.9(4) . .
O69 Mo26 O62 99.4(3) . .
O93 Mo26 O62 100.8(3) . .
O69 Mo26 O43 97.5(3) . .
O93 Mo26 O43 102.1(3) . .
O62 Mo26 O43 146.9(3) . .
O69 Mo26 O24 105.0(3) . .
O93 Mo26 O24 150.1(3) . .
O62 Mo26 O24 73.9(2) . .
O43 Mo26 O24 74.2(2) . .
O69 Mo26 O52 174.6(3) . .
O93 Mo26 O52 80.5(3) . .
O62 Mo26 O52 79.4(2) . .
O43 Mo26 O52 81.2(2) . .
O24 Mo26 O52 69.6(2) . .
O69 Mo26 Mo8 92.9(2) . .
O93 Mo26 Mo8 135.8(3) . .
O62 Mo26 Mo8 116.0(2) . .
O43 Mo26 Mo8 34.58(18) . .
O24 Mo26 Mo8 42.34(14) . .
O52 Mo26 Mo8 83.05(13) . .
O100 Mo27 O87 105.1(3) . .
O100 Mo27 O55 95.5(3) . .
O87 Mo27 O55 99.9(3) . .
O100 Mo27 O41 99.7(3) . .
O87 Mo27 O41 96.7(3) . .
O55 Mo27 O41 153.7(3) . .
O100 Mo27 O17 160.6(3) . .
O87 Mo27 O17 92.3(3) . .
O55 Mo27 O17 72.9(2) . .
O41 Mo27 O17 86.2(2) . .
O100 Mo27 O54 92.9(3) . .
O87 Mo27 O54 160.8(3) . .
O55 Mo27 O54 84.7(3) . .
O41 Mo27 O54 73.3(2) . .
O17 Mo27 O54 71.0(2) . .
O100 Mo27 Mo25 129.4(3) . .
O87 Mo27 Mo25 86.4(2) . .
O55 Mo27 Mo25 34.04(19) . .
O41 Mo27 Mo25 128.25(18) . .
O17 Mo27 Mo25 42.01(15) . .
O54 Mo27 Mo25 87.20(16) . .
O96 Mo28 O98 106.1(4) . .
O96 Mo28 O84 98.1(3) . .
O98 Mo28 O84 102.3(4) . .
O96 Mo28 O11 98.3(3) . .
O98 Mo28 O11 101.5(3) . .
O84 Mo28 O11 146.0(2) . .
O96 Mo28 O15 104.1(3) . .
O98 Mo28 O15 149.8(3) . .
O84 Mo28 O15 74.3(2) . .
O11 Mo28 O15 72.8(2) . .
O96 Mo28 O89 174.1(3) . .
O98 Mo28 O89 79.8(3) . .
O84 Mo28 O89 80.3(3) . .
O11 Mo28 O89 80.3(2) . .
O15 Mo28 O89 70.0(2) . .
O96 Mo28 Mo14 92.5(2) . .
O98 Mo28 Mo14 135.2(3) . .
O84 Mo28 Mo14 115.19(18) . .
O11 Mo28 Mo14 34.50(16) . .
O15 Mo28 Mo14 41.24(14) . .
O89 Mo28 Mo14 83.05(15) . .
O65 Mo29 O79 104.4(3) . .
O65 Mo29 O58 101.5(3) . .
O79 Mo29 O58 96.9(3) . .
O65 Mo29 O62 92.8(3) . .
O79 Mo29 O62 99.7(3) . .
O58 Mo29 O62 154.6(3) . .
O65 Mo29 O24 159.0(3) . .
O79 Mo29 O24 93.4(3) . .
O58 Mo29 O24 86.9(2) . .
O62 Mo29 O24 73.1(2) . .
O65 Mo29 O13 92.1(3) . .
O79 Mo29 O13 162.5(3) . .
O58 Mo29 O13 74.0(2) . .
O62 Mo29 O13 84.8(2) . .
O24 Mo29 O13 71.5(2) . .
O105 Mo30 O80 105.0(3) . .
O105 Mo30 O57 101.0(3) . .
O80 Mo30 O57 97.5(3) . .
O105 Mo30 O53 92.9(4) . .
O80 Mo30 O53 99.3(3) . .
O57 Mo30 O53 154.5(3) . .
O105 Mo30 O14 158.6(3) . .
O80 Mo30 O14 93.0(3) . .
O57 Mo30 O14 87.6(2) . .
O53 Mo30 O14 72.6(2) . .
O105 Mo30 O56 91.7(3) . .
O80 Mo30 O56 162.5(3) . .
O57 Mo30 O56 73.9(2) . .
O53 Mo30 O56 84.5(2) . .
O14 Mo30 O56 71.7(2) . .
O115 Mo31 O86 105.1(4) . .
O115 Mo31 O53 102.2(3) . .
O86 Mo31 O53 99.9(3) . .
O115 Mo31 O27 100.6(3) . .
O86 Mo31 O27 97.8(3) . .
O53 Mo31 O27 146.2(3) . .
O115 Mo31 O14 148.5(3) . .
O86 Mo31 O14 106.3(3) . .
O53 Mo31 O14 74.3(2) . .
O27 Mo31 O14 73.2(2) . .
O115 Mo31 Mo18 134.7(3) . .
O86 Mo31 Mo18 93.1(2) . .
O53 Mo31 Mo18 115.3(2) . .
O27 Mo31 Mo18 34.95(17) . .
O14 Mo31 Mo18 41.41(15) . .
O106 Mo32 O103 105.0(4) . .
O106 Mo32 O58 96.6(3) . .
O103 Mo32 O58 100.3(3) . .
O106 Mo32 O72 100.5(3) . .
O103 Mo32 O72 93.5(3) . .
O58 Mo32 O72 154.5(3) . .
O106 Mo32 O37 93.5(3) . .
O103 Mo32 O37 159.1(3) . .
O58 Mo32 O37 86.9(2) . .
O72 Mo32 O37 73.3(2) . .
O106 Mo32 O13 162.2(3) . .
O103 Mo32 O13 91.3(3) . .
O58 Mo32 O13 73.1(2) . .
O72 Mo32 O13 85.3(3) . .
O37 Mo32 O13 71.9(2) . .
O109 Mo33 O92 106.3(4) . .
O109 Mo33 O47 95.1(3) . .
O92 Mo33 O47 101.1(3) . .
O109 Mo33 O57 100.3(3) . .
O92 Mo33 O57 95.6(3) . .
O47 Mo33 O57 153.0(3) . .
O109 Mo33 O5 157.3(3) . .
O92 Mo33 O5 94.9(3) . .
O47 Mo33 O5 72.5(2) . .
O57 Mo33 O5 85.2(2) . .
O109 Mo33 O56 89.3(3) . .
O92 Mo33 O56 162.3(3) . .
O47 Mo33 O56 85.5(2) . .
O57 Mo33 O56 72.8(2) . .
O5 Mo33 O56 71.2(2) . .
O112 Mo34 O39 105.1(3) . .
O112 Mo34 O75 101.2(3) . .
O39 Mo34 O75 98.5(3) . .
O112 Mo34 O60 102.0(3) . .
O39 Mo34 O60 98.0(3) . .
O75 Mo34 O60 146.8(3) . .
O112 Mo34 O18 149.8(3) . .
O39 Mo34 O18 105.1(3) . .
O75 Mo34 O18 73.9(2) . .
O60 Mo34 O18 74.1(2) . .
O112 Mo34 O88 79.6(3) . .
O39 Mo34 O88 175.2(3) . .
O75 Mo34 O88 80.8(2) . .
O60 Mo34 O88 80.4(2) . .
O18 Mo34 O88 70.2(2) . .
O112 Mo34 Mo16 136.9(3) . .
O39 Mo34 Mo16 92.6(2) . .
O75 Mo34 Mo16 114.91(19) . .
O60 Mo34 Mo16 35.67(17) . .
O18 Mo34 Mo16 41.53(15) . .
O88 Mo34 Mo16 83.47(15) . .
Mo13 O1 Mo24 151.8(3) . .
Mo13 O1 Mo22 96.2(2) . .
Mo24 O1 Mo22 96.9(2) . .
Mo13 O1 Mo20 101.1(2) . .
Mo24 O1 Mo20 100.7(2) . .
Mo22 O1 Mo20 101.6(2) . .
Mo9 O2 Mo18 115.7(3) . .
Mo7 O3 Mo13 115.5(3) . .
Mo10 O4 Mo8 114.6(3) . .
Mo9 O5 Mo17 97.8(2) . .
Mo9 O5 Mo33 151.2(3) . .
Mo17 O5 Mo33 95.7(2) . .
Mo9 O5 Mo15 101.6(2) . .
Mo17 O5 Mo15 101.2(2) . .
Mo33 O5 Mo15 100.5(2) . .
Mo7 O6 Pr3 155.7(3) . .
Mo9 O7 Pr3 153.7(3) . .
Mo14 O8 Pr2 154.7(3) . .
Mo16 O9 Mo14 115.2(3) . .
Mo18 O10 Pr4 156.2(3) . .
Mo28 O11 Mo14 111.1(3) . .
Mo13 O12 Pr4 154.5(3) . .
Mo12 O13 Mo29 110.3(3) . .
Mo12 O13 Mo32 109.9(3) . .
Mo29 O13 Mo32 93.3(2) . .
Mo18 O14 Mo31 96.1(2) . .
Mo18 O14 Mo30 152.0(3) . .
Mo31 O14 Mo30 95.6(2) . .
Mo18 O14 Mo15 101.9(2) . .
Mo31 O14 Mo15 101.8(2) . .
Mo30 O14 Mo15 100.4(2) . .
Mo14 O15 Mo23 152.9(3) . .
Mo14 O15 Mo28 96.1(2) . .
Mo23 O15 Mo28 95.8(2) . .
Mo14 O15 Mo11 101.1(2) . .
Mo23 O15 Mo11 100.6(2) . .
Mo28 O15 Mo11 100.2(2) . .
Mo16 O16 Pr1 155.5(3) . .
Mo7 O17 Mo25 97.0(2) . .
Mo7 O17 Mo27 151.0(3) . .
Mo25 O17 Mo27 94.9(2) . .
Mo7 O17 Mo20 102.1(2) . .
Mo25 O17 Mo20 101.9(2) . .
Mo27 O17 Mo20 101.0(2) . .
Mo16 O18 Mo19 151.6(3) . .
Mo16 O18 Mo34 96.0(2) . .
Mo19 O18 Mo34 96.7(2) . .
Mo16 O18 Mo11 101.3(2) . .
Mo19 O18 Mo11 101.3(2) . .
Mo34 O18 Mo11 100.4(2) . .
Mo11 O19 Mo14 109.5(2) . .
Mo11 O19 Mo16 110.0(2) . .
Mo14 O19 Mo16 92.6(2) . .
Mo6 O20 Pr2 158.4(3) . .
Mo15 O21 Mo18 108.4(2) . .
Mo15 O21 Mo9 107.9(3) . .
Mo18 O21 Mo9 92.25(19) . .
Mo17 O22 Mo9 110.3(3) . .
Mo10 O23 Pr3 145.9(3) . .
Mo29 O24 Mo8 153.4(3) . .
Mo29 O24 Mo26 96.3(2) . .
Mo8 O24 Mo26 94.9(2) . .
Mo29 O24 Mo12 101.8(2) . .
Mo8 O24 Mo12 99.8(2) . .
Mo26 O24 Mo12 100.8(2) . .
Mo12 O25 Mo8 110.2(3) . .
Mo12 O25 Mo10 109.8(3) . .
Mo8 O25 Mo10 92.9(2) . .
Mo18 O26 Pr1 148.7(3) . .
Mo18 O27 Mo31 109.8(3) . .
Mo6 O28 Pr4 159.5(3) . .
Mo8 O29 Pr3 147.0(3) . .
Mo6 O30 Pr3 159.3(3) . .
Mo14 O31 Pr4 147.5(3) . .
Mo8 O32 Pr2 155.3(3) . .
Mo22 O33 Mo24 111.1(3) . .
Mo25 O34 Mo7 109.6(3) . .
Mo10 O35 Pr1 155.4(3) . .
Mo6 O36 Pr1 159.3(3) . .
Mo10 O37 Mo32 152.0(3) . .
Mo10 O37 Mo21 95.9(2) . .
Mo32 O37 Mo21 96.0(2) . .
Mo10 O37 Mo12 101.3(2) . .
Mo32 O37 Mo12 101.2(2) . .
Mo21 O37 Mo12 101.1(2) . .
Mo22 O38 Mo13 110.7(3) . .
Mo9 O40 Pr1 146.7(3) . .
Mo24 O41 Mo27 114.3(3) . .
Mo12 O42 Mo21 106.3(3) . .
Mo26 O43 Mo8 111.1(3) . .
Mo7 O44 Pr2 146.4(3) . .
Mo13 O45 Pr2 148.1(3) . .
Mo21 O46 Mo10 109.6(3) . .
Mo17 O47 Mo33 112.3(3) . .
Mo20 O48 Mo13 108.9(2) . .
Mo20 O48 Mo7 108.3(3) . .
Mo13 O48 Mo7 92.4(2) . .
Mo19 O50 Mo23 114.0(3) . .
Mo11 O51 Mo23 109.9(3) . .
Mo11 O51 Mo19 110.1(3) . .
Mo23 O51 Mo19 92.9(2) . .
Mo12 O52 Mo26 105.7(3) . .
Mo31 O53 Mo30 111.5(3) . .
Mo20 O54 Mo24 110.5(3) . .
Mo20 O54 Mo27 111.2(3) . .
Mo24 O54 Mo27 92.7(2) . .
Mo25 O55 Mo27 111.5(3) . .
Mo15 O56 Mo30 109.8(3) . .
Mo15 O56 Mo33 111.3(3) . .
Mo30 O56 Mo33 92.8(2) . .
Mo30 O57 Mo33 114.6(3) . .
Mo29 O58 Mo32 114.7(3) . .
Mo16 O59 Pr4 146.6(3) . .
Mo34 O60 Mo16 109.9(3) . .
Mo26 O62 Mo29 110.9(3) . .
Mo15 O63 Pr5 151.4(4) . .
Mo15 O63 Mo17 106.9(3) . .
Pr5 O63 Mo17 101.6(2) . .
Mo17 O71 Pr5 119.1(3) . .
Mo21 O72 Mo32 111.0(3) . .
Mo34 O75 Mo19 111.0(3) . .
Mo28 O84 Mo23 110.7(3) . .
Mo11 O88 Mo34 106.3(3) . .
Mo11 O89 Mo28 106.5(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pr1 O36 2.418(5) .
Pr1 O40 2.462(6) .
Pr1 O16 2.501(6) .
Pr1 O77 2.503(7) .
Pr1 O64 2.501(6) .
Pr1 O26 2.512(6) .
Pr1 O35 2.523(6) .
Pr1 O104 2.521(6) .
Pr1 O76 2.597(6) .
Pr2 O20 2.427(5) .
Pr2 O45 2.456(6) .
Pr2 O44 2.484(6) .
Pr2 O108 2.487(7) .
Pr2 O32 2.488(5) .
Pr2 O74 2.496(6) .
Pr2 O8 2.501(6) .
Pr2 O78 2.539(7) .
Pr2 O114 2.611(7) .
Pr3 O30 2.431(6) .
Pr3 O23 2.465(6) .
Pr3 O6 2.498(5) .
Pr3 O7 2.500(6) .
Pr3 O29 2.503(6) .
Pr3 O66 2.510(6) .
Pr3 O70 2.520(7) .
Pr3 O91 2.522(6) .
Pr3 O116 2.525(7) .
Pr4 O28 2.441(5) .
Pr4 O31 2.481(6) .
Pr4 O107 2.493(7) .
Pr4 O59 2.495(6) .
Pr4 O12 2.506(6) .
Pr4 O81 2.518(7) .
Pr4 O99 2.519(6) .
Pr4 O82 2.517(6) .
Pr4 O10 2.518(5) .
Pr5 O117 2.455(9) .
Pr5 O63 2.461(6) .
Pr5 O119 2.479(10) .
Pr5 O118 2.513(10) .
Pr5 O121 2.521(10) .
Pr5 O120 2.520(11) .
Pr5 O123 2.550(11) .
Pr5 O122 2.561(11) .
Pr5 O71 2.666(8) .
Mo6 O20 1.753(5) .
Mo6 O36 1.756(6) .
Mo6 O28 1.762(5) .
Mo6 O30 1.770(6) .
Mo7 O6 1.716(5) .
Mo7 O44 1.739(6) .
Mo7 O3 1.907(5) .
Mo7 O34 1.981(6) .
Mo7 O17 2.100(6) .
Mo7 O48 2.267(5) .
Mo7 Mo25 3.1817(13) .
Mo8 O32 1.735(6) .
Mo8 O29 1.733(6) .
Mo8 O43 1.940(6) .
Mo8 O4 1.956(5) .
Mo8 O24 2.155(5) .
Mo8 O25 2.217(5) .
Mo8 Mo26 3.1882(12) .
Mo9 O7 1.723(6) .
Mo9 O40 1.746(5) .
Mo9 O2 1.909(5) .
Mo9 O22 1.981(6) .
Mo9 O5 2.090(5) .
Mo9 O21 2.275(5) .
Mo9 Mo17 3.2004(12) .
Mo10 O35 1.731(6) .
Mo10 O23 1.745(6) .
Mo10 O4 1.896(5) .
Mo10 O46 1.983(5) .
Mo10 O37 2.129(6) .
Mo10 O25 2.256(6) .
Mo11 O89 1.738(6) .
Mo11 O88 1.744(6) .
Mo11 O19 1.888(6) .
Mo11 O51 1.904(6) .
Mo11 O15 2.252(6) .
Mo11 O18 2.263(5) .
Mo12 O52 1.725(6) .
Mo12 O42 1.744(6) .
Mo12 O25 1.884(5) .
Mo12 O13 1.906(6) .
Mo12 O24 2.248(5) .
Mo12 O37 2.259(6) .
Mo13 O12 1.719(6) .
Mo13 O45 1.744(6) .
Mo13 O3 1.949(5) .
Mo13 O38 1.951(6) .
Mo13 O1 2.119(6) .
Mo13 O48 2.252(6) .
Mo13 Mo22 3.1930(11) .
Mo14 O8 1.722(6) .
Mo14 O31 1.728(6) .
Mo14 O11 1.942(6) .
Mo14 O9 1.945(5) .
Mo14 O15 2.121(5) .
Mo14 O19 2.240(6) .
Mo14 Mo28 3.1993(12) .
Mo15 O102 1.726(6) .
Mo15 O63 1.759(6) .
Mo15 O56 1.899(6) .
Mo15 O21 1.908(5) .
Mo15 O14 2.245(5) .
Mo15 O5 2.279(6) .
Mo16 O59 1.735(6) .
Mo16 O16 1.736(5) .
Mo16 O9 1.908(5) .
Mo16 O60 1.988(6) .
Mo16 O18 2.137(6) .
Mo16 O19 2.259(6) .
Mo16 Mo34 3.2058(12) .
Mo17 O61 1.706(7) .
Mo17 O71 1.740(7) .
Mo17 O22 1.920(6) .
Mo17 O47 1.930(6) .
Mo17 O5 2.156(6) .
Mo17 O63 2.475(7) .
Mo18 O26 1.721(6) .
Mo18 O10 1.723(5) .
Mo18 O27 1.936(6) .
Mo18 O2 1.954(5) .
Mo18 O14 2.116(6) .
Mo18 O21 2.262(5) .
Mo18 Mo31 3.1811(12) .
Mo19 O85 1.729(6) .
Mo19 O68 1.730(7) .
Mo19 O50 1.936(6) .
Mo19 O75 1.996(7) .
Mo19 O18 2.149(6) .
Mo19 O51 2.253(6) .
Mo20 O101 1.736(6) .
Mo20 O90 1.740(6) .
Mo20 O54 1.896(6) .
Mo20 O48 1.914(6) .
Mo20 O17 2.264(5) .
Mo20 O1 2.276(6) .
Mo21 O110 1.706(8) .
Mo21 O111 1.723(7) .
Mo21 O72 1.934(7) .
Mo21 O46 1.927(6) .
Mo21 O37 2.173(6) .
Mo21 O42 2.496(6) .
Mo22 O67 1.715(7) .
Mo22 O113 1.724(7) .
Mo22 O33 1.931(7) .
Mo22 O38 1.930(6) .
Mo22 O1 2.171(5) .
Mo23 O73 1.695(6) .
Mo23 O97 1.727(6) .
Mo23 O50 1.946(6) .
Mo23 O84 1.983(6) .
Mo23 O15 2.164(5) .
Mo23 O51 2.240(6) .
Mo24 O83 1.722(7) .
Mo24 O95 1.727(6) .
Mo24 O41 1.925(6) .
Mo24 O33 1.989(7) .
Mo24 O1 2.150(6) .
Mo24 O54 2.246(7) .
Mo25 O94 1.714(6) .
Mo25 O49 1.724(6) .
Mo25 O34 1.913(6) .
Mo25 O55 1.923(7) .
Mo25 O17 2.146(6) .
Mo25 Mo27 3.1950(13) .
Mo26 O69 1.718(7) .
Mo26 O93 1.725(7) .
Mo26 O62 1.920(7) .
Mo26 O43 1.926(6) .
Mo26 O24 2.173(6) .
Mo26 O52 2.506(6) .
Mo27 O100 1.705(7) .
Mo27 O87 1.723(6) .
Mo27 O55 1.942(7) .
Mo27 O41 1.958(7) .
Mo27 O17 2.189(6) .
Mo27 O54 2.263(6) .
Mo28 O96 1.718(7) .
Mo28 O98 1.727(7) .
Mo28 O84 1.936(7) .
Mo28 O11 1.938(6) .
Mo28 O15 2.181(5) .
Mo28 O89 2.473(7) .
Mo29 O65 1.713(7) .
Mo29 O79 1.741(7) .
Mo29 O58 1.930(7) .
Mo29 O62 1.990(7) .
Mo29 O24 2.151(6) .
Mo29 O13 2.247(6) .
Mo30 O105 1.704(7) .
Mo30 O80 1.734(7) .
Mo30 O57 1.923(7) .
Mo30 O53 1.976(7) .
Mo30 O14 2.198(6) .
Mo30 O56 2.264(6) .
Mo31 O115 1.698(7) .
Mo31 O86 1.725(7) .
Mo31 O53 1.931(7) .
Mo31 O27 1.952(6) .
Mo31 O14 2.161(6) .
Mo32 O106 1.715(7) .
Mo32 O103 1.727(7) .
Mo32 O58 1.960(6) .
Mo32 O72 1.977(7) .
Mo32 O37 2.162(6) .
Mo32 O13 2.260(6) .
Mo33 O109 1.697(7) .
Mo33 O92 1.713(7) .
Mo33 O47 1.959(6) .
Mo33 O57 1.978(6) .
Mo33 O5 2.202(5) .
Mo33 O56 2.268(6) .
Mo34 O112 1.732(7) .
Mo34 O39 1.739(6) .
Mo34 O75 1.924(6) .
Mo34 O60 1.929(6) .
Mo34 O18 2.175(6) .
Mo34 O88 2.483(6) .
N5 N5A 0.48(9) .
N9 N9A 1.56(9) .
N11 N11A 0.69(7) .
